# “Phase Transformation in Materials”

of 33/33

date post

26-Nov-2021Category

## Documents

view

1download

0

Embed Size (px)

### Transcript of “Phase Transformation in Materials”

PowerPoint Office: 33-313 Telephone: 880-7221 Email:
[email protected] Office hours: by an appointment

2015 Fall

(Ch3) Crystal Interface and Microstructure

(Ch4) Solidification: Liquid → Solid

(Ch6) Diffusionless Transformations: Solid → Solid

Background to understand phase transformation

Representative Phase transformation

- Nonsteady-state diffusion – Fick’s Second Law

- For random walk in 3 dimensions, after n steps of length α

• Effect of Temperature on Diffusivity

: Movement of atoms to reduce its chemical potential μ. driving force: Reduction of G

Down-hill diffusion movement of atoms from a high CB region to low CB region.

Up-hill diffusion movement of atoms from a low CB region to high CB region.

(atoms m-2 s-1)

C CJ n n D x x

Concentration varies with position.

Concentration varies with time and position.

• Interstitial Diffusion / Substitutional Diffusion

• High-Diffusivity Paths 1. Diffusion along Grain Boundaries and Free Surface

2. Diffusion Along Dislocation

• Diffusion in Multiphase Binary Systems

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

- Steady-state diffusion– Fick’s First Law

- Non-steady-state diffusion: Fick’s Second Law Concentration varies with position.

Concentration varies with time and position.

5

Q. How to solve the diffusion equations? : Application of Fick’s 2nd law

homogenization, carburization, decarburization, diffusion across a couple

6

Solutions to the diffusion equations (Application of Fick’s 2nd law)

Ex1. Homogenization of sinusoidal varying composition in the elimination of segregation in casting

l : half wavelength

Initial or Boundary Cond.?

x CB

Fig. 2.10 The effect of diffusion on a sinusoidal variation of composition.

Concentrations decrease with time

Concentrations increase with time.

7

( )

( )

τ : relaxation time

D l 2

l xC πβ sin X(x,0) 0+≡DteTT

D dt

Ex1. Homogenization of sinusoidal varying composition in the elimination of segregation in casting

l xCC πβ sin0+= at t=0

τ : relaxation time

D l 2

π τ =

2 )/exp(0

lxatt =−= τββ

The initial concentration profile will not usually be sinusoidal, but in general any con- centration profile can be considered as the sum of an infinite series of sine waves of varying wavelength and amplitude, and each wave decays at a rate determined by its own “τ”. Thus, the short wavelength terms die away very rapidly and the homogenization will ultimately be determined by τ for the longest wavelength component.

decide homogenization rate Fig. 2.10 The effect of diffusion on a sinusoidal variation of composition.

Amplitude of the concentration profile (β) decreases exponentially with time,

02

2

Concentrations increase with time.

Ex2. Carburization of Steel

The aim of carburization is to increase the carbon concentration in the surface layers of a steel product in order to achiever a harder wear-resistant surface.

1. Holding the steel in CH4 and/or Co at an austenitic temperature. 2. By controlling gases the concentration of C at the surface of the steel can be maintained at a suitable constant value. 3. At the same time carbon continually diffuses from the surface into the steel.

10

Depth of Carburization?

• Since erf(0.5)≈0.5, the depth at which the carbon concentration is midway between Cs and C0 is given

that is

Solution of Fick’s 2nd law

1) Specimen ~ infinitely long. 2) Diffusion coefficient of carbon in austenite increases with increasing concentration, but an approximate solution: Taking an average value

∂ ∂ =

∂ ∂

11

Error function

In mathematics, the error function (also called the Gauss error function) is a non-elementary function which occurs in probability, statistics and partial differential equations. It is defined as:

By expanding the right-hand side in a Taylor series and integrating, one can express it in the form

for every real number x. (From Wikipedia, the free encyclopedia)

12

Schematic diagram illustrating the main features of the error function.

13

Depth of Carburization?

• Since erf(0.5)≈0.5, the depth at which the carbon concentration is midway between Cs and C0 is given

that is

Solution of Fick’s 2nd law

1) Specimen ~ infinitely long. 2) Diffusion coefficient of carbon in austenite increases with increasing concentration, but an approximate solution: Taking an average value

Fig. 2.11 Concentration profiles at successive times (t3>t2>t1) for diffusion into a semi-infinite bar when the surface concentration Cs is maintained constant.

14

Thus the thickness of the carburized layer is .

Note also that the depth of any is concentration line is directly proportion to , i.e. to obtain a twofold increase in penetration requires a fourfold increase in time.

(2 → 4 )

Ex.3 Decarburization of Steel?

Carburization

15

, 0 , 0

C C t x C C t x C C x t C C x t

Joining of two semi-infinite specimens of compositions C1 and C2 (C1 > C2 )

Draw C vs. x with time t = 0 and t > 0. Boundary conditions?

Solutions to the diffusion equations

Ex4. Diffusion Couple

Fig. 2.12 (b) concentration profiles at successive times (t2>t1>0) when two semi-infinite bars of different composition are annealed after welding.

16

The section is completed with 4 example solutions to Fick's 2nd law: carburisation, decarburisation, diffusion across a couple and homogenisation.

The solutions given are as follows:

l

Cmean = Mean concentration b0 = Initial concentration amplitude l = half-wavelength of cells t = relaxation time

Carburization CS = Surface concentration C0 = Initial bulk concentration

Decarburization C0 = Initial bulk concentration

Diffusion Couple C1 = Concentration of steel 1 C2 = Concentration of steel 2

17

Q. Interstitial diffusion vs Substitutional diffusion

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

1. Self diffusion in pure material

Probability of vacancy x probability of jump

• Interstitial Diffusion / Substitutional Diffusion

- Diffusion in dilute interstitial alloys ~ relatively simple because the diffusing atoms are always surrounded by vacant sites to which they can jump whenever they have enough to overcome the energy barrier for migration.

- In substitutional diffusion, An atom can only jump if there happens to be vacant site at one of the adjacent lattice positions

The rate of self-diffusion can be measured experimentally by intro- ducing a few radioactive A atoms (A*) into pure A and measuring the rate at which penetration occurs at various temperatures. Since A* and A atoms are chemically identical their jump frequencies are almost identical.

21 6A AD α= Γ

amenable to a simple atomic model: self-diffusion ( )

DA* =

most likely to occur back into the same vacancy

DA* = f DA ( f : correlation factor ) close to unity

Diffusion coefficient

The next jump is not equally probable in all directions.

19

Q. Interstitial diffusion vs Substitutional diffusion

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

20

1. Self diffusion in pure material

What would be the jump frequency in substitutional diffusion? An atom next to a vacancy can make a jump provided

it has enough thermal energy to overcome Gm.

The probability that an adjacent site is vacant → zXv

→ exp(-Gm/kT)

− → Γ = ν m

V GzX exp

− + = α ν2 m V

A 1 ( G G )D z exp 6 RT

For most metals: ν ~ 1013, fcc metals : z = 12, 2a=α

mGcf) zexp RT

for int erstitials

Jump frequency

A 1 ( G G )D z exp 6 RT

For most metals: ν ~ 1013, fcc metals : z = 12, 2a=α

STHG −=

~Same with interstitial diffusion except that the activation energy for self-diffusion has an extra term self-diffusion requires the presence of vacancies

22

QD D RT −

=

m m mG H T S = − 21 6B BD α= Γ

?Bjump frequency ΓThermally activated process

Ζ : nearest neighbor sites

( ) ( )

( )RTGmB /exp −Ζ=Γ ν

* interstitial diffusion

RT

Therefore, from the slope of the D-curve in an log D vs 1/T coordinate, the activation energy may be found.

How to determine QID experimentally?

Fig. 2.7 The slope of log D v. 1/T gives the activation energy for diffusion Q.

Fig. 2.14 Illustration of the principle of tracer diffusion and of the planar source method for determining the self-diffusion coefficient of gold. (a) Initial diffusion couple with planar source of radioactive gold Au*. (b) Distribution of Au* after diffusion for 100h at 920

Experimental Determination of D

1) Solution for the infinite boundary condition

M : quantity·m-2/ C : quantity·m-3

- Deposit a known quantity (M) of a radioactive isotope A*

) 4

24

(2.18)

25

For a given structure and bond type, Q/RTm is roughly constant; Q is roughly proportional to Tm.

ex) for fcc and hcp, Q/RTm ~ 18 and D(Tm) ~ 1 µm2s-1 (10-12 m2s-1)

For a given structure and bond type, D(T/Tm) ~ constant

T/Tm : homologous temperature

Most close-packed metals

Table 2.2 Experimental Data for Substitutional Self-Diffusion in Pure Metals at Atmospheric Pressure

26

* Melting point diffusivities for various classes of materials:

: The diffusion coefficients of all materials with a given crystal structure and bond type will be approximately the same at the same fraction of their melting temperature, i.e. D(T/Tm) = const.

: Since volume usually increases on melting (Tm), raising the pressure increases Tm and thereby lowers the diffusivity at a given temperature.

1. Within each class, D(Tm) ~ approximately constants.

27

: Q and Tm exhibit rough linear correlation because increasing the interatomic bond strength makes the process of melting more difficult; that is, Tm is raised. It also makes diffusion more difficult by increasing ΔHm & ΔHv.

For a given structure and bond type, Q/RTm is roughly constant;

28 < Relationship between latent heat and melting point>

b) AM ~ 1 for all liquid, AF depends on crystal structure

- Metallic structure (FCC, C.P.H, and BCC, “less localized bonding”) ~ good relationship compared with the structures which are covalently bonded (“specific directional bonds”). - Molecular liquid such as F2, Cl2 ~ extra condition for AF ( molecule must be correctly oriented in order to be accommodated.)

29

ex) At 800oC, DCu= 5 × 10-9 mm2s-1, α = 0.25 nm

2

After an hour, diffusion distance (x)? m~Dt µ4

: ?CuΓ

At 20oC, DCu~ 10-34 mm2s-1 − −Γ 20 1~ 10Cu jumps s

→ Each atom would make one jump every 1012 years!

Hint) From the data in Table 2.2, how do we estimate DCu at 20oC?

How do we determine DCu at low temperature such as 20oC?

Consider the effect of temperature on self-diffusion in Cu:

Fig. 2.7 The slope of log D v. 1/T gives the activation energy for diffusion Q.

30

Q. Interstitial diffusion vs Substitutional diffusion

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

31

All the surrounding atoms are possible jump sites of a vacancy, which is analogous to interstitial diffusion.

)/exp()/exp( 6 1

2. Vacancy diffusion

e vAv XDD /=

This shows in fact that the diffusivity of vacancy (Dv) is many orders

of magnitude greater than the diffusivity of substitutional atoms (DA).

32

JA

AB JJ ′−=′∴

* During self-diffusion, all atoms are chemically identical. : probability of finding a vacancy and jumping into the vacancy ~ equal * In binary substitutional alloys, each atomic species must be given its own intrinsic diffusion coefficient DA or DB.

33

JA

xt C AA ~

AB JJ ′−=′∴A B → +

A-rich AB B-rich AB A

net flux

: A/B

B

1

2015 Fall

(Ch3) Crystal Interface and Microstructure

(Ch4) Solidification: Liquid → Solid

(Ch6) Diffusionless Transformations: Solid → Solid

Background to understand phase transformation

Representative Phase transformation

- Nonsteady-state diffusion – Fick’s Second Law

- For random walk in 3 dimensions, after n steps of length α

• Effect of Temperature on Diffusivity

: Movement of atoms to reduce its chemical potential μ. driving force: Reduction of G

Down-hill diffusion movement of atoms from a high CB region to low CB region.

Up-hill diffusion movement of atoms from a low CB region to high CB region.

(atoms m-2 s-1)

C CJ n n D x x

Concentration varies with position.

Concentration varies with time and position.

• Interstitial Diffusion / Substitutional Diffusion

• High-Diffusivity Paths 1. Diffusion along Grain Boundaries and Free Surface

2. Diffusion Along Dislocation

• Diffusion in Multiphase Binary Systems

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

- Steady-state diffusion– Fick’s First Law

- Non-steady-state diffusion: Fick’s Second Law Concentration varies with position.

Concentration varies with time and position.

5

Q. How to solve the diffusion equations? : Application of Fick’s 2nd law

homogenization, carburization, decarburization, diffusion across a couple

6

Solutions to the diffusion equations (Application of Fick’s 2nd law)

Ex1. Homogenization of sinusoidal varying composition in the elimination of segregation in casting

l : half wavelength

Initial or Boundary Cond.?

x CB

Fig. 2.10 The effect of diffusion on a sinusoidal variation of composition.

Concentrations decrease with time

Concentrations increase with time.

7

( )

( )

τ : relaxation time

D l 2

l xC πβ sin X(x,0) 0+≡DteTT

D dt

Ex1. Homogenization of sinusoidal varying composition in the elimination of segregation in casting

l xCC πβ sin0+= at t=0

τ : relaxation time

D l 2

π τ =

2 )/exp(0

lxatt =−= τββ

The initial concentration profile will not usually be sinusoidal, but in general any con- centration profile can be considered as the sum of an infinite series of sine waves of varying wavelength and amplitude, and each wave decays at a rate determined by its own “τ”. Thus, the short wavelength terms die away very rapidly and the homogenization will ultimately be determined by τ for the longest wavelength component.

decide homogenization rate Fig. 2.10 The effect of diffusion on a sinusoidal variation of composition.

Amplitude of the concentration profile (β) decreases exponentially with time,

02

2

Concentrations increase with time.

Ex2. Carburization of Steel

The aim of carburization is to increase the carbon concentration in the surface layers of a steel product in order to achiever a harder wear-resistant surface.

1. Holding the steel in CH4 and/or Co at an austenitic temperature. 2. By controlling gases the concentration of C at the surface of the steel can be maintained at a suitable constant value. 3. At the same time carbon continually diffuses from the surface into the steel.

10

Depth of Carburization?

• Since erf(0.5)≈0.5, the depth at which the carbon concentration is midway between Cs and C0 is given

that is

Solution of Fick’s 2nd law

1) Specimen ~ infinitely long. 2) Diffusion coefficient of carbon in austenite increases with increasing concentration, but an approximate solution: Taking an average value

∂ ∂ =

∂ ∂

11

Error function

In mathematics, the error function (also called the Gauss error function) is a non-elementary function which occurs in probability, statistics and partial differential equations. It is defined as:

By expanding the right-hand side in a Taylor series and integrating, one can express it in the form

for every real number x. (From Wikipedia, the free encyclopedia)

12

Schematic diagram illustrating the main features of the error function.

13

Depth of Carburization?

• Since erf(0.5)≈0.5, the depth at which the carbon concentration is midway between Cs and C0 is given

that is

Solution of Fick’s 2nd law

1) Specimen ~ infinitely long. 2) Diffusion coefficient of carbon in austenite increases with increasing concentration, but an approximate solution: Taking an average value

Fig. 2.11 Concentration profiles at successive times (t3>t2>t1) for diffusion into a semi-infinite bar when the surface concentration Cs is maintained constant.

14

Thus the thickness of the carburized layer is .

Note also that the depth of any is concentration line is directly proportion to , i.e. to obtain a twofold increase in penetration requires a fourfold increase in time.

(2 → 4 )

Ex.3 Decarburization of Steel?

Carburization

15

, 0 , 0

C C t x C C t x C C x t C C x t

Joining of two semi-infinite specimens of compositions C1 and C2 (C1 > C2 )

Draw C vs. x with time t = 0 and t > 0. Boundary conditions?

Solutions to the diffusion equations

Ex4. Diffusion Couple

Fig. 2.12 (b) concentration profiles at successive times (t2>t1>0) when two semi-infinite bars of different composition are annealed after welding.

16

The section is completed with 4 example solutions to Fick's 2nd law: carburisation, decarburisation, diffusion across a couple and homogenisation.

The solutions given are as follows:

l

Cmean = Mean concentration b0 = Initial concentration amplitude l = half-wavelength of cells t = relaxation time

Carburization CS = Surface concentration C0 = Initial bulk concentration

Decarburization C0 = Initial bulk concentration

Diffusion Couple C1 = Concentration of steel 1 C2 = Concentration of steel 2

17

Q. Interstitial diffusion vs Substitutional diffusion

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

1. Self diffusion in pure material

Probability of vacancy x probability of jump

• Interstitial Diffusion / Substitutional Diffusion

- Diffusion in dilute interstitial alloys ~ relatively simple because the diffusing atoms are always surrounded by vacant sites to which they can jump whenever they have enough to overcome the energy barrier for migration.

- In substitutional diffusion, An atom can only jump if there happens to be vacant site at one of the adjacent lattice positions

The rate of self-diffusion can be measured experimentally by intro- ducing a few radioactive A atoms (A*) into pure A and measuring the rate at which penetration occurs at various temperatures. Since A* and A atoms are chemically identical their jump frequencies are almost identical.

21 6A AD α= Γ

amenable to a simple atomic model: self-diffusion ( )

DA* =

most likely to occur back into the same vacancy

DA* = f DA ( f : correlation factor ) close to unity

Diffusion coefficient

The next jump is not equally probable in all directions.

19

Q. Interstitial diffusion vs Substitutional diffusion

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

20

1. Self diffusion in pure material

What would be the jump frequency in substitutional diffusion? An atom next to a vacancy can make a jump provided

it has enough thermal energy to overcome Gm.

The probability that an adjacent site is vacant → zXv

→ exp(-Gm/kT)

− → Γ = ν m

V GzX exp

− + = α ν2 m V

A 1 ( G G )D z exp 6 RT

For most metals: ν ~ 1013, fcc metals : z = 12, 2a=α

mGcf) zexp RT

for int erstitials

Jump frequency

A 1 ( G G )D z exp 6 RT

For most metals: ν ~ 1013, fcc metals : z = 12, 2a=α

STHG −=

~Same with interstitial diffusion except that the activation energy for self-diffusion has an extra term self-diffusion requires the presence of vacancies

22

QD D RT −

=

m m mG H T S = − 21 6B BD α= Γ

?Bjump frequency ΓThermally activated process

Ζ : nearest neighbor sites

( ) ( )

( )RTGmB /exp −Ζ=Γ ν

* interstitial diffusion

RT

Therefore, from the slope of the D-curve in an log D vs 1/T coordinate, the activation energy may be found.

How to determine QID experimentally?

Fig. 2.7 The slope of log D v. 1/T gives the activation energy for diffusion Q.

Fig. 2.14 Illustration of the principle of tracer diffusion and of the planar source method for determining the self-diffusion coefficient of gold. (a) Initial diffusion couple with planar source of radioactive gold Au*. (b) Distribution of Au* after diffusion for 100h at 920

Experimental Determination of D

1) Solution for the infinite boundary condition

M : quantity·m-2/ C : quantity·m-3

- Deposit a known quantity (M) of a radioactive isotope A*

) 4

24

(2.18)

25

For a given structure and bond type, Q/RTm is roughly constant; Q is roughly proportional to Tm.

ex) for fcc and hcp, Q/RTm ~ 18 and D(Tm) ~ 1 µm2s-1 (10-12 m2s-1)

For a given structure and bond type, D(T/Tm) ~ constant

T/Tm : homologous temperature

Most close-packed metals

Table 2.2 Experimental Data for Substitutional Self-Diffusion in Pure Metals at Atmospheric Pressure

26

* Melting point diffusivities for various classes of materials:

: The diffusion coefficients of all materials with a given crystal structure and bond type will be approximately the same at the same fraction of their melting temperature, i.e. D(T/Tm) = const.

: Since volume usually increases on melting (Tm), raising the pressure increases Tm and thereby lowers the diffusivity at a given temperature.

1. Within each class, D(Tm) ~ approximately constants.

27

: Q and Tm exhibit rough linear correlation because increasing the interatomic bond strength makes the process of melting more difficult; that is, Tm is raised. It also makes diffusion more difficult by increasing ΔHm & ΔHv.

For a given structure and bond type, Q/RTm is roughly constant;

28 < Relationship between latent heat and melting point>

b) AM ~ 1 for all liquid, AF depends on crystal structure

- Metallic structure (FCC, C.P.H, and BCC, “less localized bonding”) ~ good relationship compared with the structures which are covalently bonded (“specific directional bonds”). - Molecular liquid such as F2, Cl2 ~ extra condition for AF ( molecule must be correctly oriented in order to be accommodated.)

29

ex) At 800oC, DCu= 5 × 10-9 mm2s-1, α = 0.25 nm

2

After an hour, diffusion distance (x)? m~Dt µ4

: ?CuΓ

At 20oC, DCu~ 10-34 mm2s-1 − −Γ 20 1~ 10Cu jumps s

→ Each atom would make one jump every 1012 years!

Hint) From the data in Table 2.2, how do we estimate DCu at 20oC?

How do we determine DCu at low temperature such as 20oC?

Consider the effect of temperature on self-diffusion in Cu:

Fig. 2.7 The slope of log D v. 1/T gives the activation energy for diffusion Q.

30

Q. Interstitial diffusion vs Substitutional diffusion

1. Self diffusion in pure material 2. Vacancy diffusion 3. Diffusion in substitutional alloys

31

All the surrounding atoms are possible jump sites of a vacancy, which is analogous to interstitial diffusion.

)/exp()/exp( 6 1

2. Vacancy diffusion

e vAv XDD /=

This shows in fact that the diffusivity of vacancy (Dv) is many orders

of magnitude greater than the diffusivity of substitutional atoms (DA).

32

JA

AB JJ ′−=′∴

* During self-diffusion, all atoms are chemically identical. : probability of finding a vacancy and jumping into the vacancy ~ equal * In binary substitutional alloys, each atomic species must be given its own intrinsic diffusion coefficient DA or DB.

33

JA

xt C AA ~

AB JJ ′−=′∴A B → +

A-rich AB B-rich AB A

net flux

: A/B

B

1